Department of Physics, Harvard University, Cambridge, Massachusetts 02138, United States Department of Chemistry and Chemical Biology, Harvard University, Cambridge, Massachusetts 02138, United States § Department of Physics, Oklahoma State University, Stillwater, Oklahoma 74078, United States ‡

S Supporting Information *

ABSTRACT: Raman scattering plays a key role in unraveling the quantum dynamics of graphene, perhaps the most promising material of recent times. It is crucial to correctly interpret the meaning of the spectra. It is therefore very surprising that the widely accepted understanding of Raman scattering, i.e., Kramers−Heisenberg−Dirac theory, has never been applied to graphene. Doing so here, a remarkable mechanism we term“transition sliding” is uncovered, explaining the uncommon brightness of overtones in graphene. Graphene’s dispersive and ﬁxed Raman bands, missing bands, defect density and laser frequency dependence of band intensities, widths of overtone bands, Stokes, anti-Stokes anomalies, and other known properties emerge simply and directly.

KEYWORDS: Raman spectroscopy, quantum chemistry, resonance theory, theoretical chemistry, UV−vis spectroscopy

T

opinion that DR was a wrong turn on the way to understanding graphene quantum dynamics and Raman spectroscopy. When KHD is applied to graphene, phonons are produced exclusively and instantly at the moments of photoabsorption or photoemission by the explicit nuclear coordinate dependence of the transition moment. The transition moment in DR fourth-order perturbation theory expression is taken to be a constant. It has already been noted that a nonconstant transition moment is needed to understand some aspects of nanotube spectroscopy.2 The present graphene study has a strong precedent in another conjugated conducting polymer. In a recent study,3 the long-standing mysteries of the dispersive polyacetylene Raman spectrum yielded to KHD theory, extended to include 1-D crystal structure, defects, and electron and phonon dispersion relations. All these arise from within Born−Oppenheimer theory and KHD Raman scattering theory. The coordinate dependence of the transition moment plays a key role, since geometry does not change when the electron−hole pairs are created in the extended conjugated system. These principles are the starting point for surprising new insights that graphene has in store. For example, “transition sliding”, not possible in a DR picture, is responsible for the brightness of overtone bands, and explains their impurity and

he unique properties of graphene and related systems have propelled it to a high level of interest for more than a decade. Raman scattering is perhaps the key window on graphene’s quantum properties, yet the crucial aspects of the spectrum of graphene, carbon nanotubes, and graphite Raman spectra have been a subject of much controversy, in some cases for decades. The delay in applying Kramers−Heisenberg−Dirac theory (KHD) to graphene is attributable to the rise of a nontraditional, fourth-order perturbative Raman model (KHD is second order) called “double resonance” (DR), which appeared 15 or so years ago,1 rapidly gaining wide acceptance exclusively in the conjugated carbon Raman community. DR is not a variant of KHD tuned to graphene, but rather it is incompatible with KHD. DR relies on inelastic electronic scattering to create phonons, requiring introduction of two additional orders of electron−phonon perturbation theory, making it overall fourth order. These inelastic processes make no appearance in KHD, which cleanly produces phonons free of Pauli blocking by two other mechanisms, overall in second order perturbation theory. Search engines quickly reveal that none of the 3000+ published contributions developing DR or using it to interpret experiments has mentioned the much older and more established KHD Raman formalism, in the last 15 years. No rationale was ever given as to why a radically diﬀerent, nonKHD formalism was needed. On the face of it, even without regard to the theory given in this paper, these facts leave the DR approach seriously unexamined and exposed. It is our © 2016 American Chemical Society

Received: December 16, 2015 Accepted: January 22, 2016 Published: January 22, 2016 2803

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818

Article

www.acsnano.org

Article

ACS Nano doping dependence, as well as their disappearance in the deep UV. Transition sliding does not apply to polyacetylene because there are no Dirac cones and no linear dispersion; indeed polyacetylene overtones are correspondingly weak.

Σiρ→, σf =

8π e 4ωs3ωI 9c 1 ℏ

αi ,ρf , σ =

RESULTS AND DISCUSSION Does the Born−Oppenheimer Approximation “Break Down” for Graphene? KHD relies heavily on the Born− Oppenheimer approximation, as does much of condensed matter physics. Recently, the “headlines” in a highly cited paper left the impression that the ABO fails particularly in graphene. The excellent article has the provocative title “Breakdown of the adiabatic Born−Oppenheimer approximation in graphene”.4 Published in Nature Materials with over 800 citations, we ﬁnd the statements “... ABO has proved eﬀective for the accurate determination of chemical reactions, molecular dynamics and phonon frequencies in a wide range of metallic systems. Here, we show that ABO fails in graphene.” and later “Quite remarkably, the ABO fails in graphene”,4 see also ref 5. Born−Oppenheimer is an approximation and fails in speciﬁc regimes and situations. Reference 4 claims nothing very drastic once one reads deeper. Instead it makes important points about a stiﬀening of the G mode with electron density near the Dirac point involving the Kohn anomaly, missed by ABO. By their nature, Kohn anomalies involve rapid changes of electronic structure with small nuclear conﬁguration changes, a warning sign of potential ABO breakdown. In this paper, we do not attempt to correct for the Kohn anomalies and their eﬀect on phonon modes and mode frequencies. Electron−hole pairs created in Raman studies are normally well away from the Dirac point and orbitals aﬀected by Kohn anomalies. The ABO succeeds in the large, that is, the point. Recall that within ABO, if the nuclei return to a prior conﬁguration, the electrons do also. This is strictly incompatible with inelastic electron−phonon scattering having taken place in the meantime. Inelastic electron−phonon scattering is nonetheless a valid nonadiabatic correction to ABO. However, electron− phonon scattering would appear to Pauli block the aﬀected electrons, immediately rendering them silent in Raman scattering. We have been given a late opportunity to use KHD theory the ﬁrst time in graphene. KHD is vastly more established than DR, and astonishingly accurate most of the time. It much simpler to execute, and lower order in perturbation theory. Kramers−Heisenberg−Dirac Theory. We provide a review of KHD here; facilitating the developments in succeeding sections. Just before the dawn of quantum mechanics, in 1925 Kramers and Heisenberg published a correspondence principle account of Raman scattering,6,7 which Dirac translated into quantum form in 1927.8 The Kramers− Heisenberg−Dirac Theory of Raman scattering has been used ever since to explain more than half a million Raman spectra in a very wide range of systems, including very large conjugated hydrocarbons. There is no reason that removing hydrogens from carbon materials should cause KHD to catastrophically fail and require replacement by a theory based on diﬀerent physics. The KHD formula for the total Raman cross section Σ, for incident frequency ωI and polarization ρ, scattered frequency ωs and polarization σ, between initial Born−Oppenheimer state |i⟩ and ﬁnal Born−Oppenheimer state |f⟩ via intermediate Born−Oppenheimer states |n⟩ reads

4

|αi ,ρf , σ |2 ;

⎡ ⟨f |D† , σ |n⟩⟨n|D ρ|i⟩ ⎣ Ei − En + ℏωI − i Γn

∑⎢ n

⟨f |D |n⟩⟨n|D ρ|i⟩ ⎤ ⎥ Ei + En + ℏωI + i Γn ⎦ †,σ

+

(1)

where Γn is the damping factor for the excited state, accounting for events and degrees of freedom not explicitly represented. The transition moment operator D controls the ﬁrst-order perturbative matter−radiation coupling. Usually the second, nonresonant term inside the square in eq 1 is neglected, for simplicity. Making this more explicit, suppose with phonon coordinates ξ and electron coordinates r, we write |f ⟩ = |ψmB . O .(ξ , r)⟩ = |ϕ(ξ ; r)⟩|χm (ξ)⟩, f

f

|i ⟩ =

|ψmB . O .(ξ , i

|n⟩ =

|ψqBq. O,.m(ξ , v c

r)⟩ = |ϕ(ξ ; r)⟩|χm (ξ)⟩, and i

r)⟩ = |ϕq q (ξ ; r)⟩|χm (ξ)⟩ v c

vc

(2)

|ϕ(ξ;r)⟩ is the approximation to the Born−Oppenheimer π electron ground state (we suppress the other electrons) based on a Slater determinant of valence electron spin orbitals; |ϕqvqc(ξ;r)⟩ is an electron−hole pair relative to the ground state, with an electron in the conduction band orbital |ϕqc(ξ;r)⟩ and a hole in the valence band orbital |ϕqv(ξ;r)⟩. |ϕqvqc(ξ;r)⟩|χmvc(ξ)⟩ is a complete intermediate state, including the phonon wave function. qv, qc and mvc may range quite freely, with the following remarks: (1) almost all qvqc, mvc will give vanishing matrix elements with the dipole operator, due to momentum nonconservation (including the momentum of the phonons). (2) Some pairs qvqc with unmatched momentum qv ≠ qc give nonvanishing matrix elements nonetheless because they are associated with newly created or destroyed phonons contained in |χmvc(ξ)⟩ relative to the initial state, conserving momentum. Such states are the electron−hole-phonon triplets. (3) Momentum is conserved when elastic backscattering is required to realign the hole and particle (because of the kick given to the conduction electron by newly formed or destroyed phonons) through the recoil of the whole sample, or laboratory, as is familiar in Mössbauer scattering or elastic neutron scattering for example. This feature is embedded in eq 2 since the electronic orbitals include the presence of impurities, edges, etc., which are part and parcel of ABO. Even though the eigenfunction orbitals thus include the elastic backscattering as a boundary condition entirely within ABO, and thus opposite momenta are populated, we may decompose the process of promotion into opposite traveling components. Promoting one propagation direction, the electron is kicked to the opposite by the phonon production at 2q−. But the opposite direction is already occupied, in the valence state. Therefore, elastic backscattering is still required in spite of the mixed nature of the orbitals. Time is required for this to happen. In the energy domain, being oﬀ resonance in eﬀect shortens the time and nearly removes the eﬀects of the backscattering. Due to dilution of the delocalized π orbital amplitude over the inﬁnite graphene sheet, it is almost obvious that the Born− Oppenheimer potential energy surface is unchanged after a 2804

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818

Article

ACS Nano

coordinates, i.e., the Placzek polarizability, would vanish without coordinate dependence of the transition moment. If the transition moment is (unjustiﬁably) set to a constant independent of phonon coordinates, no Raman scattering occurs at all in KHD theory for graphene. The intermediate, typically conduction band (assuming no doping) Born−Oppenheimer states |ψB.O. qvqc,m(ξ,r)⟩ with energy Ev,c,m range over resonant and nonresonant (very small or not so small denominators, respectively) states including all with nonvanishing matrix elements in the numerator. Only those with Pauli and momentum matched electron−hole pairs and electron−hole−phonon triplets can be nonvanishing; it is not necessary that they be “resonant”, i.e., minimize the denominator, in order to contribute importantly (however, see caveats below to modes like D requiring backscattering). Rather, a range of states is collectively important, the range depending on Γ. Although not relevant to undoped graphene, even when none of the denominators reach resonance, there is still suﬃcient Raman amplitude to be quite visible as oﬀ resonance Raman scattering. The ﬁnal Born−Oppenheimer state |χmf(ξ)⟩ with energy Emf conserves total system plus incident and emitted photon energy, and may diﬀer from the initial state only by 0, 1, 2, ... phonons. The electron has ﬁlled the hole and the initial electronic state is restored. An exception to this notation is the ﬁlling of an empty level created by doping, leaving the hole created by the photon unﬁlled. All the electronic states reside exactly on the electronic band surface, here on the Dirac cone near the Dirac point. It is good to keep in mind that the vast majority of states |ϕqvqc(ξ;r)⟩|χmvc(ξ)⟩ (violating momentum conservation with respect to the initial state for example) in the KHD sum have vanishing matrix elements and do not lead to Raman (or even Rayleigh) scattering. Some terms (or really a small group of terms, see discussion in section “Kramers−Heisenberg−Dirac Theory” about backscattering) give nonvanishing matrix elements, and if they include phonons, they are usually still incapable of Raman emission. An example is a D phonon produced in absorption in a clean sample, unable to emit a Raman photon due to the Pauli blocking eﬀect of the electron recoil. Such states eventually relax and thermalize by a cascade of e−e and e−ph inelastic processes. Sliding transitions (see the section “Sliding Phonon Production”) do not help because even elastic backscattering by defects does not alleviate the Pauli blocking for the majority D phonons produced. These “orphan” phonons, not appearing in the Raman spectrum, are always in the majority compared to phonons seen in Raman emission. It is not the phonons themselves that fail (they live on quite well), but rather their associated, Pauli-blocked conduction electrons than cannot emit to signify the phonon via a Stokes shift for example. Even if no phonon is produced at the time of absorption, the chances of achieving Rayleigh emission are small, or phonon production upon emission even smaller, given the withering removal of electrons from eligibility by inelastic e−e scattering, raising the near certain specter of Pauli blocking. This occurs on a femtosecond time scale (see refs 9−13). Phonon Adjusted Electronic Transitions. A fraction of resonant conduction band eigenstates |ϕqvqc(ξ;r)⟩|χmvc(ξ)⟩ giving nonvanishing matrix elements diﬀer by one or more phonons relative to the valence band state. The energy of the Born−Oppenheimer eigenstates is a sum of phonon and electronic components, so the largest, resonant terms in the KHD

single electron−hole pair excitation from the ground electronic state. No new forces on the nuclei arise upon a single electron− hole pair formation and no geometry changes take place, thus, the independence of |χmvc(ξ)⟩ on the electron−hole state denoted by qvqc (the occupations indicated by vc may vary, but the phonon wave functions themselves do not depend on the electron−hole pair created). The Transition Moment Operator. We may write ⟨n|D ρ|i⟩ = ⟨χm (ξ)|⟨ϕq q (ξ ; r)|D ρ|ϕ(ξ ; r)⟩|χm (ξ)⟩

(3)

⟨n|D ρ|i⟩ = ⟨χm (ξ)|μqρ, q (ξ)|χm (ξ)⟩

(4)

vc

v c

as vc

c

v

with ρ

μqρ, q (ξ) = ⟨ϕq (ξ ; r)|D̂ (r)|ϕq (ξ ; r)⟩r c

v

c

(5)

v

The matrix elements of the dipole operator D between two Born−Oppenheimer electronic states is the transition moment μρqc,qv(ξ) connecting valence level qv and conduction band electronic levels qc. μρqc,qv(ξ) is written for light polarization ρ; the subscript r indicates that only the electron coordinates are integrated. Note that μρqc,qv(ξ), if it does not vanish, is explicitly a function of phonon coordinates ξ. In terms of the transition moments, the Raman amplitude reads (using only the resonant term of the two) αmρi,,σmf =

1 ℏ

⎡ ⟨χ (ξ)|μσ (ξ)† |χ (ξ)⟩⟨χ (ξ)|μ ρ (ξ)|χ (ξ)⟩ ⎤ qv, q c m m q c, qv mi ⎢ mf ⎥ ⎢ ⎥ Emi − Ev , c , m + ℏωI − i Γj , m v ,c ,m ⎣ ⎦

≡

1 ℏ

⎡ ⟨φ (ξ)|χm (ξ)⟩⟨χm (ξ)|φq , q , m (ξ)⟩ ⎤ c v i ⎢ qv, q c, m ⎥ ⎢ ⎥ Emi − Ev , c , m + ℏωI − i Γq , m v ,c ,m ⎣ ⎦

∑ ∑

j

(6)

The sum over the intermediate states with energy denominators is of course the energy Green function, i.e., the Fourier transform of the time Green function propagator. Although we do not write out the time dependent expression here (see Supporting Information), we see that the valence state phonon wave f unction |χmi(ξ)⟩ arrives in the conduction band multiplied and thus modif ied by the transition moment μρqj,q(ξ), including its phonon coordinate dependence, before any time propagation takes place. Moreover, that propagation does not f urther change the phonon populations. The product of the transition moment and the phonon wave function is called φqj,q,mi(ξ) above. When φqj,q,mi(ξ) is reexpanded in all the phonon modes |χm(ξ)⟩ in all the conduction bands, some m will diﬀer in the occupation numbers compared to the unmodiﬁed initial lattice occupation mi (recall that because there is no geometry or force constant change, the phonons are the same in all valence and conduction bands). Every electron−hole pair production event carries some amplitude for no phonon change, plus simultaneously a ﬁnite amplitude for phonon creation or destruction relative to the initial phonon wave function. The transition moment’s dependence on nuclear separation or equivalently phonon displacements is unquestionable, not only on direct physical grounds and explicit calculations, but also because there would be no oﬀ-resonant Raman scattering without it. The derivative of the polarizability with nuclear 2805

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818

Article

ACS Nano

Figure 1. (A) Phonon creation in absorption, with diminished electronic energy. (A1) The electron wave vector q is lowered to q−, aﬀecting the phonon energy through its dispersion. The blue transition represents the photon energy. νD is the eﬀective frequency of the diminished transition. (A2) Defect elastic backscattering allows matched electron−hole (no Pauli blocking) Raman Stokes emission. (B) Stokes D band phonon creation in emission. (B1) Full absorption of the photon by the electron−hole pair. (B2) Defect induced elastic 2q backscattering of the conduction band electron, allowing Raman Stokes emission and D(2q) phonon production perfectly matched with the hole. The energies of the D phonons produced in absorption and emission diﬀer, according to q− versus q and the dispersion of the D band. Anti-Stokes scattering (not shown) proceeds very similarly, except augmentation rather than diminishment applies.

provided it creates a phonon at −2q at that precise moment of emission (due to coordinate dependence of the transition moment). The emitted light must be of the proper Raman shifted frequency to conserve energy. The processes described are shown in Figure 1B. Since in this case q did not suﬀer diminishment in absorption, it will produce a phonon with slightly larger magnitude −2q (no “−” on the q is present) than if produced in absorption with its diminished transition. The Raman shifts are thus slightly diﬀerent depending on whether the phonon was created at the time of emission or absorption, since given dispersion the phonon will have a slightly diﬀerent energy with a diﬀerent q. This means that all entries in phonon dispersion diagrams made based on the DR model needs a small correction, because absorption electron−hole−phonon triplet transitions are not at the q DR supposes, diﬀering instead by a phonon energy and the eﬀect of dispersion. Reich remarks: “To ﬁnd the doubleresonant q we assume that the q = 2ke rule is strictly valid.”14 The correction we think is needed is small, and contributes to the broadening (the addition of for example q and q− peaks) as well as slight shift of the center frequency. The terms in the KHD sum constructively and destructively interfere with one another before the square is taken. The sum includes many diﬀerent momentum conserving electron−hole pairs and electron−hole−phonon triplets leading to the same ﬁnal states of the graphene system. Processes leading to diﬀerent ﬁnal states (e.g., a diﬀerent ﬁnal phonon type or energy) appear in separate, noninterfering terms. Avoiding Pauli Blocking. An important pathway that avoids Pauli blocking begins with q−c = −q−v , associated with a phonon of pseudomomentum k = 2q−v , where the superscript “−” refers to a diminishment of the electronic transition energy by the simultaneous creation of a 2q− phonon (in the case of Stokes scattering); see below. The conduction electron suﬀers a q−v → −q−v kick to conserve momentum, and is Pauli-blocked. However, in this case, subsequent defect elastic backscattering can realign it with the hole, allowing recombination. A photon is emitted at a frequency revealing the diminished Stokes shift of the 2q− phonon production. Since the diminished q− depends also on the incoming laser energy, the phonon dispersion will be revealed by changing that energy. A 2q− modulation of the G mode for example will become Raman allowed by this mechanism. The modest dispersion of that mode will give rise to a sideband to G, which we call Gs, visible

sum eq 2 necessarily arrive with the electronic transition energy correspondingly lowered if a phonon is activated in the conduction band eigenstate relative to the valence state or raised if a phonon is deactivated in the conduction band eigenstate relative to the valence phonon wave f unction. This key fact automatically alters electronic transition energies and phonon f requencies for dispersive bands. For phonon creation, the valence energy of the hole is raised, and the conduction band energy lowered, keeping q the same in both, thus creating momentum matched (possible except needing elastic backscattering) holes and particles free of Pauli blocking. We term this prepayment a “diminished” electronic transition in the case of phonon creation (leading to Stokes scattering), and an “augmented” electronic transition in the case of phonon annihilation (leading to anti-Stokes scattering). It is important to note (see also the section “Virtual Processes and Backscattering”) that it is very diﬃcult to produce an electron−hole triplet (i.e., with a phonon change) oﬀ-resonance in a mode requiring backscattering. Thus, the dispersive modes are locked into a given diminishment or enhancement depending on the laser energy. Near resonance, the pseudomomentum q− is determined by the requirement that the energy cost of creating the electron− hole−phonon triplet is just the laser photon energy. Typically, most of the energy needed is electronic, on the order of 1.5 eV or more with the phonon energy on the order of several 0.1 eV, which is not ignorable. The electronic transition energy is given by Ee = Ec(q−) − Ev(q−) = hνI − Ephonon(2q−), where superscripts c, v refer to conduction and valence bands. As hνI is changed, q− of the phonon changes according to the valence and conduction band dispersion, which ideally is a Dirac cone structure with light-like linear dispersion of both bands. As q− changes, the phonon energy Ephonon(2q−) changes according to the well-known positive dispersion of about 50 cm−1/eV for the D band, see Figure 1A. For simplicity, we usually use intravalley diagrams even when (in some cases) the process is intervalley. If in a single phonon transition the phonon is created or destroyed at the time of emission, the electron−hole pair formation is not diminished or enhanced. All the initial photon’s energy goes into the electronic transition, as in DR, and no phonon change is yet present. The momenta of electron and hole are created in a matched pair (again, near resonance) with pseudomomentum q. The conduction band electron may then elastically backscatter q → −q, in the presence of defects. This allows recombination with the hole of momentum q, 2806

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818

Article

ACS Nano

Figure 2. (Left panels) The extended tight binding results for the G and Gs modes. The valence states are at the far left. The middle panel (on the left) depicts the conduction band state in each case, and at the top right of the left set of panels is shown the derivative of the transition moment with respect to the k = 0 G phonon coordinate, and the k = 2q Gs (formerly called D′; see below) phonon coordinate (bottom right of the left set of panels). (Middle panel) The ﬁrst derivative of the transition moment in the D sideband mode direction at K + q,

K = 2π

(

1 1 , 3a 3 3 a

), q = 2π(0,

1 12 3 a

). The transition moments and their derivatives are integrals over the data in these ﬁgures. The ﬁrst

derivative of the transition moment has amplitude of 1.2 in arbitrary units. (Right panel) The second derivative of the transition moment, which has amplitude 0.01.

distances r can be extracted and its empirical formula at the linear order reads:

only in the presence of defects. This is exactly what is observed, see Figure 3. Another important case is q−v = q−c , i.e., k = 0, which was discussed in the section “The Transition Moment for Graphene”. This corresponds to creating a Γ point G phonon that carries no momentum, but it still carries energy. Some of the photon’s energy is channeled directly into the G phonon energy, diminishing the (in the case of Stokes scattering) electron−hole transition energy, including shifting the |q| of the transition nearer to the Dirac cone K point, as if lower energy light had been used: 0.185 eV lower for a 1500 cm−1 phonon. Raman emission is active because the electron and hole are born matched in q and ready to recombine. Fast e−e scattering is the enemy of Raman emission, since if it occurs, the change in electron momentum makes Pauli blocking a near certainty. (Studies point to a time scale of a few femtoseconds before irreversible relaxation of conduction band electrons by e−e scattering. Deﬁnitive experimental results9−13 aﬃrm the extremely rapid relaxation of photo excited electrons due to e−e scattering.) The G band is indeed bright, and beneﬁts too from oﬀ resonant contributions (unlike D), but the fact that a normally weak overtone, 2D, is perhaps 10 times brighter than G follows from a fascinating process; see section “Sliding Phonon Production” below on sliding transitions. Tight Binding and Density Functional Realization of Graphene KHD. The simplest model Hamiltonian for the single-layer graphene involves only nearest-neighbor interactions. However, in the presence of crystal distortions, the hopping strength should vary with the pair distance. This is especially important to incorporate here, since this will contribute to the dependence of transition moments on geometry changes, needed in our KHD theory. On the basis of the DFT band structure and Bloch waves, the Kohn−Sham Hamiltonian can be transformed into a basis of maximally localized Wannier functions (MLWF)15 using the Wannier90 code. The initial projections for Wannier functions are the atomic pz orbitals and the transformed Hamiltonian is the ab initio tight-binding Hamiltonian. By varying the positions of the basis atoms, the hopping strength t for diﬀerent pair

t(r ) = t(r0) + f1 (r − r0)

(7)

where r0 = 1.42 Å, t(r0) = −2.808 eV and f1 = 5.058 eV/Å. Figure 2 gives the extended tight binding results for the G and Gs modes at the left, in two three-panel strips, one above the other. The middle panels of each strip depict the conduction band states, and the rightmost panels show the derivative of the transition moment with respect to the k = 0 G and the k = 2q Gs phonon coordinate, shown by the small arrows within the images (notice the undulations in the atomic displacements). The middle and right panels show the ﬁrst and second derivatives of the transition moments for the D mode at K + q, where K = 2π

(

1 1 , 3a 3 3 a

), q = 2π(0,

1 12 3 a −

).

Consider a transition from K + q (valence) to K − q− (conduction), with K = 2π

(

1 1 , 3a 3 3 a

), q

−

(

= 2π 0,

1 12 3 a

). K

is exactly at the Dirac cone, q gives a small displacement from the cone center, a is the carbon−carbon bond length at equilibrium. In this case, the electron has a momentum change of −2q−, and the phonon has momentum 2q−. (For comparison, using the graphene sheet only partly depicted in Figure 2, the constant part of the transition moment has amplitude about 60 in arbitrary units). With displaced atoms of amplitude 0.01 Å (adjusted according to 2q− modulation), the ﬁrst derivative of the transition moment has amplitude of 1.2; the second derivative has amplitude 0.01. We ﬁnd that the electronic transition moment has a robust ﬁrst derivative along any choice of the independent and degenerate G mode phonon coordinates, and this accounts for their presence in the Raman spectrum. Figure 2 shows the local transition moment along one of those choices. It is seen to be perfectly repetitive with the unit cell translation vector as beﬁts a k = 0 optical mode. Integration of this 2D local transition moment over space yields the transition moment at the given nuclear positions, and repeating this after a phonon distortion reveals the phonon coordinate dependence of the transition moment. 2807

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818

Article

ACS Nano

Figure 3. (Left) Averaged defective graphene 12C Raman spectrum on a Si substrate, adapted with permission from ref 16. Copyright 2012, American Physical Society. (Right) Placement of phonon dispersion points found and assigned through Raman spectroscopy by Hilke et al.,16 reproduced with permission. Copyright 2012 American Physical Society. D′ symbol replaced by Gs, appropriate to a sideband of G.

Thus, D should be robust (with suﬃcient elastic backscattering), but simultaneous production of 2D seems in doubt. Since 2D is the brightest band, an explanation is needed, and is given below in the section labeled “Sliding Phonon Production”; see also the evidence for them, “Hole Doping Evidence of Sliding D Absorption”. Analysis of Graphene Raman Band Structure with KHD. We now go though a few prominent characteristics of graphene Raman spectrum discovered and discussed over the years. All can now be explained (very directly) by the KHD theory. In Figure 3 a Raman spectrum obtained by the Hilke group is an average of 60 diﬀerent samples, each with defects, in order to bring out weak bands forbidden in clean, perfect graphene crystals. The D band is one such case, while 2D is allowed and bright in pure samples. Origin of G Band Intensity. The constant part of the electronic transition moment for arbitrary electronic q is nonvanishing and responsible for most of the light absorption in graphene. It delivers electrons to the conduction band without creating a phonon. A phonon’s creation (or annihilation) is the result of a changing electronic transition moment as its coordinate is displaced from equilibrium. The more rapid the change in transition moment as a function of phonon coordinate, the more likely is the phonon’s creation. The G modes have no dispersion; the same q = 0 mode is produced independent of laser frequency. The G mode may also be produced in emission. The KHD expression has the same transition moment promoting either event. The production of the G by either means is a small minority of events in any case, as is any phonon producing a successful Raman emission. (It is often stated that typically only about 1 in 1011 or 1012 incident photons causes a Raman emission.) The mechanism based on KHD for G mode production in absorption is given in Figure 4. In the section “G Mode Brightening”, we discuss the brightening of the G mode band due to hole doping and oﬀ resonant scattering. For the G-mode, the phonon production oﬀ resonance occurs by the same mechanisms familiar in KHD that populate vibrational modes in smaller systems oﬀ resonance. Virtual Processes and Backscattering. The G mode does not require backscattering to be produced. The electron is ready to ﬁll the hole the moment in appears. Not so the D mode. To produce a D mode, a momentum-conserving recoil

Figure 4. Production of a G phonon in absorption, according to KHD extended to graphene.

of the conduction electron is required. For that mode to be visible in Raman emission, the Pauli-blocked electron must be elastically backscattered. Oﬀ-energy shell virtual processes are by nature short-lived; forcing the conduction electron to ﬁll the hole quickly and emit a Raman shifted photon. This leaves insuﬃcient time for oﬀ shell elastic backscattering. Any oﬀresonant electron and hole cannot remain long, since after some time the energy imparted becomes more certain; oﬀresonance, the energy is not suﬃcient to support this. The diﬃculty is seen in the eq 6. If an oﬀ resonance state is created with a phonon and qv = −qc, in a pure sample without subsequent backscattering this situation arrives Pauli-blocked at the second transition moment operator, and the numerator vanishes, which should be taken as evidence that no virtual process will intervene. However, the Born−Oppenheimer approximation is comfortable with boundary conditions like walls and scatterers and if they are present, the Born− Oppenheimer propagation will time evolve some of say a righttrending electron wave into a left-trending one. Even for an embedded impurity, some of the scattering built into the Born−Oppenheimer propagation will be elastic backscattering. This amplitude arrives at the second transition moment operator and matrix element survives, i.e., it is not Pauliblocked. Absence of 2G Overtone. Given the robust strength of the G band, at least a small overtone at 2G would be expected, yet the 2G band did not make any appearance in the spectra of Hilke et al.,16 where other weak bands were seen for the ﬁrst 2808

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818

Article

ACS Nano

same, the sliding transition amplitudes all share the initial state |i⟩ and ﬁnal state |f⟩ and add coherently, before the square is taken. The energy Ev,c,m in the sum over electron−hole− phonon triplets |ϕqvqc(ξ;r)⟩|χmvc(ξ)⟩ is not changed by sliding: the same photon is absorbed, and always put into making the same −2q− phonon with the balance put into the electronic part of the transition; thus, Ev,c,m is highly degenerate. The initial state is the ground electronic state with no hole, no conduction electron, and no phonon change; the ﬁnal state also has no hole, no conduction electron, but if it has given a Raman shift, it has phonons (usually one or two) added or subtracted from the initial state. The initial and ﬁnal state remain the same for all the sliding intermediate states, which therefore interfere with each other. The sliding diagram in fact describes the intermediate state, including the hole that is created, the conduction electron, and the phonon. Even though we think of the electron as being promoted from valence to conduction band, this happens as a change to the ﬁxed initial state; the hole does not deﬁne the initial state, rather it is part of what deﬁnes the intermediate state. The sliding transitions are already built into the KHD eq 2; one has only to examine the possible intermediate states to see that they are present. Their ultimate limitation will be a topic for future study: trigonal warping and distortion away from linear dispersion at energies farther from the Dirac point will cause slightly diﬀerent energy phonons to be produced; these will add to the intensity noncoherently, only after the square. They will broaden the transition but are intrinsically less bright due to diminishing constructive interference. Also limiting the sliding is the density of states, diminishing to 0 as the band edges are reached. We have checked the transition moments for sliding transitions with our tight binding model. For example, we examined the transition from an occupied conduction band level at K + q to an empty conduction band at K + 3q. The transition moment ﬁrst derivative is not signiﬁcantly smaller than a transition from an occupied valence band at K − q to an empty conduction band at K + q. Sliding adds to the transition amplitude for production of the ﬁrst 2q− phonon, but electrons produced by such sliding transitions do not match the holes they leave behind and are thus Pauli-blocked in emission. Elastic backscattering does not rescue these phonons from obscurity; (K + q− + δq, backscattered elastically, gives K − q− − δq, which does not match the original hole at K − q− + δq). Below, we note hole doping creates empty valence bands, that can, if conditions are right, accept emission from such conduction band states, giving rise to a spectacular broadband “electronic Raman” emission as seen in reference;17 see “Hole Doping Evidence of Sliding D Absorption”. (These authors provided a diﬀerent interpretation involving “hotband” emission following electron−phonon scattering.) Reversing the Path. The Raman-silent single phonon sliding can become Raman active if the conduction band electron, produced by a sliding transition along with a k = 2q− phonon, emits (without ﬁrst backscattering) to the valence band along the reverse path used in absorption (see Figure 5). A second, oppositely propagating phonon is released. The electron is automatically matched to the hole and recombines, without Pauli blocking of any sort, and in the case of D phonons, a proper matched 2D phonon pair has been produced. The cumulative eﬀect of constructively interfering

time. We have been touting the uncommon strength of the overtones in graphene, so this absence must be regarded as one of its mysteries and must be explained. There is no group theoretical ban on its existence, and like G, it is a Γ point mode, requiring no backscattering. Why is it missing? DFT-tight binding calculations of the transition moment show that the second derivative along the G phonon mode is about 2 orders of magnitude smaller than the ﬁrst derivative. Since the intensity goes as the square of the transition moment, this would wash out 2G if it were the only scenario for a 2G. However, there is another possibility to consider: The robust linear slope in the transition moment along the G mode could be used twice, once in absorption and the second time in emission. Although not a simultaneous production of the phonons, two G mode phonons will have been produced, and a Raman band would appear at 2G. The phonons together would be pseudomomentum k = 0. It is easy to see however that the intensity for this process must be extremely low: If there is an amplitude of 0.025 (probably much too high an estimate, but conservative for this purpose) for producing a single G mode in absorption, the amplitude for two G phonons, one in absorption and one in emission, is 0.000625. This corresponds to a probability of two G phonons produced this way some 1600 times smaller than the probability of a single G phonon production. “One up, one down” does not lead to a visible signal. Paradoxically, we will see that this “one up, one down” mechanism is the key to the brightness of the 2D band, and other overtone bands. The 2G mode is unable to increase its brightness by one up, one down “transition sliding” (see the section “Sliding Phonon Production”), because sliding requires a k = 2q phonon be produced. Sliding greatly ampliﬁes the chance of producing a phonon, for example in the case of 2D, or 2Gs (formerly called 2D′) since many simultaneous amplitudes are summed. Transition sliding is a key principle made possible by linear Dirac cone dispersion (see the section “Sliding Phonon Production”), and a key Raman mechanism revealed here. The Gs [Former D′] and 2Gs [Former 2D′] Bands. Nearby the Γ point k = 0 phonon, the transition moment can also give rise to k = 2q− phonons, giving a momentum kick 2q− to the conduction band electron. Elastic backscattering makes recombination possible, revealing the existence of the sideband to G formerly known as D′, now Gs, The healthy 2Gs band, present without impurities, is the overtone of defect-hungry Gs band. Published spectra are often cut oﬀ before its ca. 3200 cm−1 displacement is reached. Its frequency is very close to twice that of Gs. It seems the 2Gs band owes its unexpectedly large intensity in the absence of defects to the same transition sliding mechanism that beneﬁts 2D; see the next section. Sliding Phonon Production. The brightness of the 2D overtone mode (and of other k = 2q overtone bands like 2Gs) is a consequence of continuously many simultaneous transition amplitudes, all producing the same D phonon in absorption and one of opposite pseudomomentum in emission. Amplitude for electron−hole and electron−hole−phonon production appears simultaneously up and down the Dirac cone, vastly extending the nominal symmetrical K − q to K + q transition (giving a −2q kick to a new phonon). That is, a continuum of K − q− + δq to K + q− + δq transitions is available, all generating the same −2q− phonon. This is possible due to the linear dispersion of the Dirac cone. Since the 2q− phonons are the 2809

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818

Article

ACS Nano

probability of producing a pair of D phonons. The density of states for both the initial and ﬁnal electronic states will have a major eﬀect on the propensity to slide various amounts. The sliding mechanism explains many known facts of Raman scattering in graphene. First and foremost, the brightness of the 2D and other overtone bands (mixed transitions can also occur, i.e., two phonons each from a diﬀerent band, as long as the pseudomomentum of both is the same). As just explained, this results from addition of a continuous range of sliding amplitudes, before the square is taken to give Raman intensity. The fact that the 2D peak strongly decreases with increasing doping or disorder is now explained easily: Doping can provide much faster phonon-less emission pathways emptying conduction band levels and diminishing the population producing emission of another D phonon. Moreover, scattering of the conduction electron (it does not have to be elastic backscattering) by defects will also quench the D emission probability by Pauli blocking. The D phonons produced in absorption are present nonetheless; the electron is hung up in the conduction band and must relax by means other than Raman emission. D Band Stokes, Anti-Stokes Anomaly. The Stokes versus anti-Stokes frequencies in the D and 2D bands are graphene Raman anomalies, discussed ﬁrst in pyrolytic carbon19,20 and graphite whiskers.18 There are two striking experimental results to explain: (1) A diﬀerence between D band Stokes and antiStokes frequencies. In a small molecule, the Stokes and antiStokes bands measure the same vibrational state, and there cannot be any diﬀerence between the two: they are symmetrically spaced across the Rayleigh line, i.e., 0 asymmetry. For the graphene D band, the asymmetry is instead about 8 or 9 cm−1. (2) As shown in the next section, the 2D band Stokes, anti-Stokes asymmetry is not twice the D band asymmetry, which would be expected because two D phonons are produced, but close to 4 times the D band shift, or 34 cm−1. These numbers emerge simply from our KHD theory, without invoking any virtual processes. The D mode Stokes band is an average of emission and absorption production, with emission production unshifted.

Figure 5. Transition sliding on a Dirac cone. (Left) The nominal, symmetric “Double D” (2D) transition with energies equal above and below the Dirac point. Absorption is followed, without any backscattering, by emission along the reverse path, producing a second phonon of opposite momentum. (Right) By moving the rectangle up, not changing any dimension, we ﬁnd it still ﬁts absorption and emission transitions (it could also slide downward) along the Dirac cone. The reference transition is shown as a dashed rectangle. Sliding the rectangle up or down leaves the phonon 2q− unchanged.

such amplitudes over a continuous sliding range of terms in the KHD sum (the numerator is absolute value squared of the sum of all sliding terms producing the same pair of phonons,). This produces a large enhancement of the 2D Raman band intensity. In graphite whiskers, the intensity of the 2D overtone is found to be about 10 times stronger than the single phonon G mode, normally expected to be much stronger than an overtone band.18 As mentioned above, the G or 2G modes are not amenable to sliding transitions. Figure 5 shows the sliding scenario. A large range of sliding ΔEv = ΔEc, i.e., equal shifts in valence and conduction bands, are available; all of these are resonant, not virtual, transitions. Compared to the reference, nonsliding symmetric case, in upsliding the valence wave vector has been shortened by δq, and the conduction wave vector has been lengthened by the same amount, so it remains a 2q− transition and gives a 2q− phonon production, just as when δq = 0. All the sliding transitions are independent amplitudes at the same photon energy simultaneously present, and together, they vastly enhance the

Figure 6. Predictions of Stokes and anti-Stokes Raman spectra of the D and 2D band positions and their anomalies, in KHD theory. The horizontal scale of the 2D-band spectra (upper right) spans twice the range of the D scale. Anti-Stokes processes were brought across the origin of the Rayleigh line and are shown dotted. See text for details. 2810

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818

Article

ACS Nano

Figure 7. (Top) Response of polyacetylene and graphene Raman spectra to defects, boundaries, and laser frequency. Figure adapted with permission from ref 25, Figure 2, for nanographite (Copyright 2006, American Institute of Physics); ref 3, Figures 4 and 5, for polyacetylene (Copyright 2015, American Chemical Society), and ref 26, Figure 9, for graphene (Copyright 2013, Nova Science Publishers, Inc.).

Production in absorption is shifted down 8 cm−1, by the dispersion of D and the diminishment cause by energy conservation. The average of the two is 4 cm−1 closer to the Rayleigh line than the undiminished emission production alone would be (see Figure 6). Similarly, the D mode anti-Stokes production in absorption also consists of two bands, overall 4 cm−1 higher in energy and farther from the Rayleigh band. At 3.5 eV and 1350 cm−1, the Stokes vs the anti-Stokes D phonons (reﬂected about the Rayleigh line for comparison) will diﬀer by about 8.4 cm−1. This is an anomalous Stokes, anti-Stokes asymmetry of about 8.4 wave numbers, in excellent agreement with experiment. Thus, the anomaly has a simple explanation in terms of phonon production in absorption vs emission. The 2D Band. The 2D overtone band in pure graphene is the strongest line in the spectrum, even much stronger than the fundamental G band. The Kohn anomaly has been proposed as a contributor to the strength of 2D, and indeed it may be, but then G is weaker, also born at a Kohn anomaly, and is a fundamental, not a normally weak overtone. It is important to note that if two counter-propagating D phonons were actually produced simultaneously in absorption, there would be a doubling (two phonons) of a double

diminishment of the electronic energy (since twice the energy is needed from the photon to produce both phonons at once). This implies a shift of 32 cm−1 relative to the presumably equally important simultaneous emission production of two counter-propagating phonons, a transition that is not diminished in energy or q. This would imply that the 2D band would either be double or a single peak considerably broader than 32 cm−1. This would not be consistent with experiments revealing a slightly asymmetric line about 25 cm−1 fwhm.21 But there is another possibility, just described, that of producing a D phonon in absorption and another in a mirror image emission. There are a continuum of such amplitudes which can slide up and down the cone, part of the KHD sum, each contributing an imaginary part with the same sign to the total 2D amplitude and each producing phonons at the same 2q− pseudomomentum (see Figure 5). The simultaneous 2D production in emission or absorption with its 32 cm−1 problem is thus alleviated (not to mention it is very weak compared to what sliding produces). The sliding mechanism also predicts the experimentally measured Stokes-anti-Stokes anomaly for 2D (see below). The density of states for both the initial and 2811

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818

Article

ACS Nano ﬁnal electronic states will have a major eﬀect on the propensity to slide various amounts. 2D Band Stokes, Anti-Stokes Anomaly. The 2D Stokes, anti-Stokes anomaly is simple to explain. In the sliding mechanism, both phonons share the same energy and diminishment, or augmentation (in anti-Stokes). Each Stokes D (one in absorption, one in emission) suﬀers an 8.4 cm−1 diminishment, or 17 cm−1 total, and each anti-Stokes D enjoys an 8.4, cm−1 augmentation, or 17 cm−1 altogether, for an overall 34 cm−1 asymmetry, four times greater, not the expected two times greater, than the 8.4 cm−1 D band asymmetry. Again, this is in agreement with experiment (see Figure 6). The D and 2D Stokes, anti-Stokes anomalies are thus directly and simply explainable using KHD theory, unlike the very elaborate rationales used to coax the DR model to agree.19 D and 2D Bandwidths; 2D Intensity with Laser Frequency. The D-mode band must be broader than the band centers spaced by 8 or 8.4 cm−1 that comprise it. We ﬁnd it to be ca. 20−25 cm−1 fwhm in the literature, about twice the fwhm of the G mode, or 13 cm−1.5 The G has no dispersion and no issues of Stokes, anti-Stokes anomalies. A D line much broader than 13 cm−1 supports the idea that the Stokes D mode is really the superposition of two displaced peaks, one coming from production in absorption, another in emission. Not only are the Stokes and anti-Stokes peaks shifted by 8.4 cm−1; they also must be overlapping when brought to the same side of the Rayleigh peak, exactly as seen in experiment; see also Figure 6. The 2D bandwidth is only somewhat larger than D, approximately 30 cm−1. It is not a double peak, at least not until the symmetry is broken (as revealed by tensioning the sample in some direction). It seems likely that 2D earns its width in a diﬀerent manner than D, perhaps a result of the sliding process on slightly nonlinear or trigonally warped Dirac cones. Intensity Changes with Frequency in 2D and G. The decrease in 2D intensity with increase laser energy, and broadening of 2D, leading to near complete absence of 2D at 266 nm in the ultraviolet,22 is easy to explain based on the KHD and sliding transition picture. The graphene electronic dispersion suﬀers signiﬁcant bending (as distinct from trigonal warping) as the ultraviolet is approached, degrading the linearity essential to the coherent sliding 2D mechanism and its interference enhancement. It is easy to show the sliding is nowhere linear at 266 nm. On the other hand, the G mode frequency is insensitive to the laser energy increase, since it does not depend on transition sliding for its intensity. It has been reported to increase intensity at the fourth power of the laser frequency,22 which ﬁts the ωIω3S classic KHD dependence, eq 1. G is ready to emit a Raman shifted photon immediately upon photoabsorption, and beneﬁts from oﬀ-resonance contributions. Defect and Laser Frequency Trends. Several interesting trends develop in the Raman spectra as density of defects or laser frequency changes. We begin with the fascinating similarity of sidebands in polyacetylene and graphene. High symmetry k = 0 dispersionless bands can be parents of dispersive sidebands carrying momentum 2q−, coming from the production of a phonon in absorption, where q− is slightly less than q, the higher electronic pseudomomentum when no phonon is produced. The conduction band electron gets kicked to −q− as it generates a 2q− phonon. If −q− is populated initially, that is not the hole waiting to be ﬁlled; rather q− is. Therefore, elastic backscattering is required to appear in the

Raman signal. In emission, the sideband phonons carry momentum 2q. The trends in the Gs band are quite parallel to sidebands in polyacetylene: ﬁxed k = 0 peaks with nearby dispersive sidebands, growing in intensity with increasing sources of elastic backscattering, and moving in frequency according to the band dispersion and phonon q. The Gs band (formerly called D′) has nothing to do with the D band, and is simply the sideband to G, as Hilke16 and others have known for some time. Sideband Growth with Impurity Density. The growth in sideband intensity with increasing sources of impurity backscattering is seen on the left of Figure 7.23 We explained these trends entirely within a KHD context applied to the onedimensional polyacetylene crystal with defects.3 The sideband growth shown in the 1054 cm−1 polyacetylene band as elastic backscattering defects are added is seen at the upper left in Figure 7. The ﬁgure was adapted and the k = 0 band contribution colored, using Schäfer-Siebert et al.23 The sideband is present at 0% added defects because of pre-existing defects (including molecular ends). The total intensity consists of the k = 0 band and the overlapping sideband, making a break in slope to the right of the k = 0 band peak. At the top right, an important graphene Raman study taken from Childres et.al.24 is shown, with permission, with similar sideband growth (Gs, sideband to G). Trends with laser frequency in sideband growth and dispersion as a function of incident laser frequency are shown at the lower left for polyacetylene and graphene (red arrows in the case of polyacetylene, giving band frequency predictions based on electron and phonon dispersion and backscattering trends with laser frequency3). The trend is opposite in the two cases. In graphene, the conductance trend is toward increased sideband strength with decreasing laser energy, as seen in Figure 7. In polyacetylene, the trend is reversed. One obvious eﬀect causing this diﬀerence is that a propagating electron wave cannot fail to collide with a defect in one-dimensional polyacetylene. We have undertaken density functional calculations on polyacetylene distorted by kinks and other geometrical defects, which show that higher energy electronic states backscatter more readily from such defects than do lower energy ones, in the conduction band. In Figure 7, both polyacetylene and graphene show increased sideband intensity as edges or ends grow closer to the interior, increasing the eﬃciency of elastic backscattering. The D and 2D Bands Are Sidebands to “DK”, a Forbidden k = 0 K Point Vibration. In a deﬁnable sense, the D and 2D bands are dispersive sidebands in a classic way to a nondispersive, but forbidden Dirac K point band we call DK, living at the vibrational K-point. In another classic case, the dispersive bands Gs [D′] and 2Gs [2D′] are sidebands to the nondispersive G band, see Figure 7. In still another classic case, dispersive sidebands in polyacetylene3 are partner to visible nondispersive bands belonging to Γ point vibrations. The band edge K point vibration DK is of course not a Γ point vibration; one consequence is that it has a vanishing transition moment and Raman intensity, as is required by symmetry. This however does not disqualify the D and 2D bands from being labeled as dispersive sidebands to the silent and dispersion-less DK parent band; DK would lie typically 8 cm−1 to the left of D and not require backscattering. Defects and 2D Intensity. There is a well-known dramatic decrease in the 2D band intensity with increased defect 2812

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818

Article

ACS Nano density27 (Figure 7, upper right). This is easily understood in terms of the sliding production of the two D phonons. The amplitude for production of the ﬁrst D phonon in absorption is relatively insensitive to defect density. Transitions with no sliding contribute to D Raman intensity if they are elastically backscattered, and indeed the D intensity increases with added impurities. Sliding D transitions are Pauli-blocked, even if backscattered, since their wave-vector mismatch with the hole persists. Sliding transitioned electrons are equally prone to defect elastic backscattering or more often, general scattering, making it extremely unlikely they can produce another D in emission, being unable to reverse absorption path. Defect scattering of the conduction electron thus quenches the source of D phonon production in emission, and the 2D Raman band intensity diminishes as defects are added. This is just what is seen in Figure 7. The reverse trends of D and 2D intensity with added defects therefore follow from the sliding, “up and back down along a reversed path” mechanism for 2D Raman emission. Anomalous Spacing of D and 2D. A prediction can be made about the D, 2D spacing seen in experiments at any frequency. This has been discussed within the DR model also.19,28 The frequency of 2D is smaller than twice D, by amounts depending on experimental conditions. The ideal “bare,” unstrained, low temperature, and fairly clean (but dirty enough to see D) graphene experiment has not been done to our knowledge. However, quoting Ding et.al.,28 “The results show that the D peak is composed of two peaks, unambiguously revealing that the 2D peak frequency (ω2D) is not exactly twice that of the D peak (ωD). This ﬁnding is conﬁrmed by varying the biaxial strain of the graphene, from which we observe that the shift of ω2D/2 and ωD are diﬀerent.” According to our application of KHD to graphene, a 1335 cm−1 D phonon produced in absorption is diminished owing to the 50 cm−1/eV phonon dispersion, by 1335/8065 × 50 = 8.28 cm−1. A D phonon produced in emission is undiminished. The two bands will overlap to make a broader feature than either component. Assuming the two bands are equally intense, as KHD predicts, there should be a combined band with an average 4 cm−1 displacement to the left in the Stokes spectrum. The idea that D is composed of two bands with an 8 cm−1 splitting was also suggested within the DR model,19 with a very diﬀerent justiﬁcation, “depending on which of the intermediate states is virtual”.20 The reason for the two bands is actually much less exotic (absorption vs emission production) and on a ﬁrmer foundation in KHD (both real, resonant processes) than the virtual processes supposed in DR. The 2D band consists of two separately produced, diminished D phonons. There is an 8 cm−1 diminishment in absorption, and a matched 8 cm−1 diminishment in emission according to the sliding scenario, totaling a 16 cm−1 shift. As just discussed, the D band is displaced by 4 cm−1, thus twice the frequency of D is predicted to be 8 cm−1 shifted as opposed to the 16 cm−1 shift of 2D, or a −8 cm−1 diﬀerence between 2 × D and 2D. Review of many published spectra under diﬀerent conditions shows E(2D) − 2E(D) ∼ −2 to −10 cm−1. However, samples were suspended on diﬀerent substrates by a variety of methods; measured shifts depend on these conditions. Reference 28 shows that any source of stretching or compression can aﬀect the D, 2D distance. The D, 2D shift deserves more investigation using suspended, gently pinned graphene.

Mixed Bands and Bandwidth Trends. Does the sliding mechanism enhancing the 2D band brightness also contribute to the strength of other bands? We have already noted that sliding does not help the D band gain intensity, since the electron is Pauli-blocked even with elastic backscattering (however, see the last section for the changed situation when the sample is hole doped). The G band transition cannot slide since the Γ point produces a k = 0 phonon. The same applies to 2G, which does not appear in the Raman spectrum regardless of defects. The sliding mechanism for mixed transitions is a diﬀerent story than for homogeneous ones, especially for bandwidth. The momentum conservation requirements on the production of a pair of phonons requires that they are matched in q. They do not need to be matched in type; e.g., a Raman band for Gs (old D′) and D3 (Hilke’s notation) could be produced by the sliding mechanism. This fact allows us to explain many of the disparate bandwidths seen in the Hilke et.al. data,16 since diﬀerences in dispersion and frequency of the two components contributes to the bandwidths, as we presently see. Most of the mixed transitions are weak (and certainly would be invisible without transition sliding), as Figure 3 shows. The weakness may reﬂect small transition matrix elements or the possibility of destructive interference between terms in the sum in eq 1. The strength of homogeneous two phonon transitions, like 2D or 2Gs, is expected to be high since they are produced by mirror image processes with in-phase numerators. For mixed transitions, sliding applies but leads to slightly diﬀerent Raman band frequencies depending on which phonon is produced ﬁrst, in absorption. The bandwidth will reﬂect this (see Figure 8). Using data from Hilke16 at 288 nm, we arrive at Figure 8. The reasons for the bandwidths of the D + Gs and 2D + Gs are discussed below. Red stars on D + D″ and Gs + D″:

Figure 8. Calculated (blue) and experimental (data from ref 16, red) bandwidths for mostly mixed combination bands. The calculations were as follows: The wavenumber diﬀerence for Gs (old D′) up ﬁrst and D4 down versus D4 up ﬁrst and Gs down was calculated using the mode frequencies and dispersion slopes from ref 16. The Raman shift (and phonon energies) depend on which transition is ﬁrst, and this diﬀerence is widening the bands. For modes a and b, the formula is W = (|Sa − Sb|)(ℏωa + ℏωb) where W is the component of the width coming from which mode is created ﬁrst, Si is the dispersion slope in cm−1/eV, and ℏωi is the energy of the phonon in eV. The theoretical results are compared to widths found in the data from ref 16 after adding 16 cm−1 for the “intrinsic” width. Except for the Gs + 2D (assignment and data taken from ref 29) and Gs + D, the agreement is good, and it lends conﬁdence to the KHD approach and the one up, one down scenario double phonon. See text for discussion of bands labeled by a red star. See Supporting Information for a discussion of the “outliers” in the sense of a poor ﬁt, indicated by black stars. 2813

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818

Article

ACS Nano

Figure 9. Continuum emission in graphene from normally Pauli-blocked sliding transitions at some laser energies and hole dopings. Horizontal bands are spaced by 0.1 eV. At the top, four scenarios for doping levels and sliding transitions at 1.58 eV laser energy are shown, together with their relation to the data of ref 17. For a D phonon, the diminished electronic part of the transition is at 1.41 eV = 1.58 eV (laser energy) − 0.166 eV (phonon energy). Scenario 1 at 2|EF| = 1.1 eV is Pauli-blocked without defect backscattering; sliding does not help; and is therefore invisible in Raman. Scenario 2 at 2|EF| = 1.1 eV is shown sliding down 0.15 eV, thus matching a hole opened by doping and avoiding Pauli blocking. However, is produces a minimum 3765 cm−1 electronic Stokes shift (lower dashed line). Scenario 3 at 2|EF| = 1.4 eV is within the bright continuum electronic Stokes emission starting at ca. 1340 cm−1 and going higher, but cut oﬀ at higher Stokes shifts by (1) declining density of states as the relevant conduction and valence bands approach the Dirac point, and (2) the emission factor ω3s (see eq 1). Scenario 4 (upper dashed line) needs to slide down to reach occupied levels that can be promoted to the conduction band, but this again causes large Stokes shifts. Scenario 5 applies to a hypothetical 2.18 eV laser energy (not used in the hole doping experiment of ref 17); it shows that at any available hole doping, the D + electronic Raman shift continuum emission would not appear anywhere near the low energy regime seen in the current experiment. The complete fading out of the 2D band at the onset of the continuum emission (lower right) as 2|EF| is increased is explained in the text. The panel at lower right is adapted with permission from ref 17. Copyright 2011 Nature Publishing Group.

Raman shift) is slightly diﬀerent if A is created in absorption than if B is. This fact contributes to a small uncertainly in frequency and contributes to the bandwidth. We calculated the bandwidths for each mixed transition and added 16 cm−1 to allow for the intrinsic broadening seen in narrow bands, due presumably to phonon decay.4,31 Using data mostly from Hilke16 at 288 nm, we arrive at Figure 8. Hole Doping Evidence of Sliding D Absorption. Chen and co-workers17 hole doped the valence band by as much as 0.8 eV and saw abundant continuum emission, in a certain range of depletion and Raman shift. We now show this emission, that as ref 17 points out, integrates to more than 100 times the strength of the G band that it overlaps, can be explained by sliding D phonon transitions that are normally Pauli-blocked or could have been the ﬁrst step in making a 2D pair by reversing the sliding transition, coupled with an electronic Raman component. With hole doping, D phonons produced in a sliding transition and the associated electronic conduction band level are normally orphaned by Pauli blocking (unless the electron returns by the sliding 2D mechanism along the reverse path). With deep doping the electron has a new option: to emit to a

We have used ref 30 to help understand the skewed line at about 2450 cm−1 with the nominal assignment D + D″. This study decomposed it into two bands, one of which is D + D″ with a width of 20 cm−1, and the overlapping higher energy LO Gs band near the Γ point, but now near the K point, a less intense band, with a fwhm of 29 cm−1. Some mixed sliding transitions, such as Gs + D3, Gs + D4, and even some hint of D + D5 (Hilke’s notation, except D′ → Gs) do not require defect backscattering and are seen weakly in high quality spectra of clean graphene, for example in Childres et al.26 Consider a mixed overtone band involving phonon modes A and B. If A is created in absorption, the q−A of the transition will be diﬀerent than if B is created ﬁrst, giving an electron pseudomomentum q−B . If A is a higher frequency phonon than B, the electronic transition energy diminishment is larger if A appears in absorption, and q−A will be smaller. The emission B phonon must follow with the opposite pseudomomentum 2q−A . This allows for matched electron−hole recombination, but the B phonon is required to adjust its energy to arrive at the right qA−. This energy correction depends on its momentum dispersion. Thus, the total phonon energy (and thus the 2814

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818

Article

ACS Nano

Figure 10. Mostly nonresonant electronic processes contributing to G mode creation, including under hole doping. See text.

valence orbital emptied by doping without creating another phonon. The original hole remains unﬁlled, and the valence orbital emptied by doping is ﬁlled instead. This leads to a continuum of potentially large electronic Stokes shifts. (Electronic Stokes because the valence electron has been promoted, not a phonon in the ﬁnal step.) This phononless emission step is far more likely than creating another phonon, and thus, the “feedstock” of the 2D band is depleted, quenching the 2D band. The 2D band should fade out in the experiment as the continuum emission appears, just as seen in the experiment (see lower dotted white line, Figure 9). Before that happens, we note that deeper hole doping lessens the sliding up distance available before the last populated initial valence level is reached. This progressively removes sliding 2D transitions, weakening the 2D band as 2|EF| increases. The consistent, progressive weakening of the 2D starting as low as 2|EF| = 0 is evident in the lower right experimental data. G Mode Brightening. In the paper by Wang and his group,17 a brightening of the G band is noted as hole doping is increased. It can be seen as a gradual waxing of G intensity in Figure 9, even after the continuum band is exceeded in the upper left corner of the plot on the lower right. The authors attributed this to removal by doping of destructively interfering paths. We agree: this also happens within the KHD picture. The sum over nonresonant states |n⟩ of energy En normally extends above and below resonance, which causes cancellations in the real part of the sum. Doping eliminates part of the sum on the high side of resonance, enhancing the real part. The relevant states |n⟩ all contain matched electron−hole G phonon triplets and matched electron−hole pairs (if G is to be produced in emission, with slightly diﬀerent energy denominator) even if En is quite nonresonant In Figure 10, case A, a given laser frequency causes below (1) and above (3) resonant transitions capable of instant production of a G mode, and a resonant one (2). Emission energy is reduced by the same energy in each case by the same G phonon produced, so the cases (1), (2), (3) add coherently. In the below resonance Raman transition (1), virtual promotion occurs from the lower blue solid to the upper

blue dashed line. Due to momentum conservation, no other states are available (they give zeros in the numerator of the KHD sum) starting at the blue valence level. The upper blue dashed state is an electron−hole−phonon triplet. Since the phonon is produced instantly, there is no time-energy roadblock to forming a G mode. All three cases apply to the same incident photon. (B) With hole doping, some transitions are no longer possible with their valence levels “missing”. This eliminates some coherent destructive interference of terms in the KHD sum. (C) The G mode phonon coordinate is displayed as the abscissa, and energy in the ordinate. Filled bands are solid; empty bands are dashed. The density of states is indicated qualitatively using the level spacing. The restriction red-to-red, blue-to-blue is due to q-conservation (small energy diﬀerences due to phonon production not shown). A continuum of oﬀ-resonant transitions apply for the same laser energy (arrows are the same lengths) and the same phonon. The sum over such states is truncated wth hole doping and the above resonance missing terms have the opposite sign in their real part with below resonance terms still present. Thus, some of the cancellation present without hole doping is lifted, enhancing G intensity, in agreement with ref 17. When present, real (not virtual) processes play a dominant role in KHD, and apart from hole or particle doping scenarios, real pathways are always available in graphene. Virtual processes (such as those present in ordinary oﬀ-resonant Raman scattering) do not normally play a center stage role, living in the shadows of the real, resonant processes, contributing mostly near resonance, in accordance with damping factors. Oﬀ-resonant (pre- or post-resonant) Raman scattering still contributes in parallel with resonant transitions in graphene, just as it does in molecular systems. For hole doped graphene, oﬀ-resonant transitions may dominate when the resonant initial valence states are depleted of population. For example, starting on the lower Dirac cone below a hole doped, lowered EF, a laser may be too low in energy to reach resonant levels on the upper cone (see Figure 10, B); yet, electron−hole excitation and recombination with no Pauli blocking quickly follow upon virtual absorption, within a time scale Δt given by the detuning 2815

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818

Article

ACS Nano ΔE from resonance, where ΔtΔE ∼ ℏ/2. A G phonon, for example, may thus be created or destroyed, oﬀ resonance. Time can become too short for electron−phonon scattering or any nuclear motion to develop; these go no faster than t1 (time after absorption), but Raman intensity comes instead from an instantaneous, t0 phonon creation/annihilation process, which KHD provides through the transition moment coordinate dependence.

METHODS The Transition Moment for Graphene. Consider the integral involving transition between a valence Bloch orbital at pseudomomentum qv, described in terms of Wannier functions αqv(r − Rqv(ξ)), and a conduction Bloch orbital at pseudomomentum qc, assuming only nearest neighbor (A with nearest B) interactions. The transition moment becomes μqρq (ξ) = v c

∑ ∫ dre−iqv·RA(ξ)αA(r − RA(ξ))D̂ ρeiqc·RB(ξ)αB(r − R B(ξ)) A, B

CONCLUSION

+ c. c.

The universally used (except in the conjugated carbon community), 90 year old KHD Raman scattering theory has been applied for the ﬁrst time in graphene Raman scattering. The results are in excellent agreement with experiment, and new insights (and predictions about new hole doping experiments) have resulted. The most important of these may be the sliding transitions, explaining the brightness of overtone transitions in graphene. KHD includes nuclear coordinate dependent transition moments as a central part of the theory. The coordinate dependence becomes crucial when nuclear forces do not change in making an electronic, photoinduced transition. DR keeps transition moments constant; in fact, DR bypasses KHD completely. Instead, ad hoc, one or two orders of perturbatively treated, Born−Oppenheimer violating electron−phonon scattering are inserted. Virtual processes are ﬁnally needed to create phonons in the conduction band. The result is a fourth-order perturbation theory, two orders beyond KHD. If we take photoabsorption and electron−hole formation to be real, and suppose that electron−phonon scattering takes time, then conduction electron energy and momentum is well established before inelastic scattering. This all-resonant picture leads straight to severe Pauli blocking after the kick and energy reduction the electron receives in inelastic electron−phonon scattering. The fact that Raman scattering is in fact robust in graphene leads the DR model to suppose instead that nonresonant virtual processes must have lead to a ﬁnal “double resonance” and provided the Raman photons. But now that we know the transition moment coordinate dependence, combined with all-resonant processes free of Pauli blocking provide the Raman photons, the appeal to virtual processes and inelastic electron phonon scattering becomes unnecessary. Ockham’s razor would strongly suggest taking the simpler, resonant, real, lower order in perturbation theory, long established KHD theory seriously. We believe KHD is the correct theoretical basis for understanding Raman scattering in graphene. Using KHD, in one contribution we have been able to explain the major eﬀects discovered in 15 and more years of experimental eﬀort on graphene and graphite, including the behavior of ﬁxed and dispersive Raman bands, their dependence on laser frequency, their sensitivity to defect and doping densities, anomalies in Stokes, anti-Stokes positions and widths, hole doping experiments, brightness of 2D and absence of 2G, widths of diﬀerent overtone features, and more. We have exposed the sliding mechanism, a direct result coordinate dependence of the transition moment and linear Dirac cone dispersion. A key spectroscopic agent in graphene, sliding is plain to see in the KHD formula. Sliding explains graphene’s extremely bright overtone bands.

3

=

∑ e−i(qv− qc)·RA(ξ) ∑ eiqc·δj⃗(ξ)DAρ,Bj(ξ) j=1

A

≡

∑e

−i(qv − q c)·RA(ξ)

- ρ(q c, A, ξ)

A

(8) δ⃗j(ξ) is a nearest neighbor vector, i.e., Bj = A + δ̃j(ξ). qv,qc are Bloch pseudomomenta in the valence and conduction band, respectively. Here we have given only the simplest form of the transition moment; in fact, in our calculations, we use density functional theory modiﬁed Wannier wave fuctions as a function of nuclear coordinate; see the section “Tight Binding and Density Functional Realization of Graphene KHD”. The sum and therefore the transition moment vanishes at the equilibrium position of the lattice ξ0 unless qv = qc or qv − qc = K, a reciprocal lattice vector, since - ρ(q c , A, ξ0) is the same function of qc for all A. However, it is not the transition moment at a single conﬁguration of the nuclei that is required, but rather the integral over phonon matrix elements, i.e., eq 4. Suppose qv = qc, so we are considering a Γ point vibration. Clearly the exponential is unity. But it is easily seen that ∂- ρ(q c , A, ξ)/∂ξG ≠ 0 at ξ = ξ0, i.e., - ρ(q c , A, ξ0) is odd at ξ0 about either G mode. (Moving the A lattice up slightly and the B lattice down by the same amount is a distortion along a G mode Γ point vibration.) Thus, the transition moment can induce changes by one quantum (and also more, we do not analyze that here) in the G modes, at the Γ point. A phonon of pseudomomentum k = qv−qc can be induced by lattice distortion ξk ≠ ξ0 and the transition moment if μqρq (ξk) = ∑A e−i(qv − q c)·RA(ξk)- ρ(q c , A, ξk ) becomes nonvanishing v c

for qv − qc = k or qv − qc = k ± K. This happens due to periodic undulations in - ρ(q c , A, ξk ) arising from displacement of the lattice RA(ξk) and RB(ξk) according to a phonon with wave vector k. However, unless strict conditions are met, such phonons, though present, are associated with a conduction band electronic level that is Pauli-blocked, keeping the phonon silent in the Raman spectrum. Elastic backscattering will not help, except for special cases, as described next. If hole doping is present, matters can be changed in a fascinating way; see “Hole Doping Evidence of Sliding D Absorption’. Ab Initio Procedure. A two-step ab initio procedure is used to model realistic hopping parameters, computing transition moments and their coordinate dependence. First, the density functional theory (DFT) calculations are performed using the Vienna ab initio Simulation Package (VASP)32,33 with the exchange-correlation energy of electrons treated within the generalized gradient approximation (GGA) as parametrized by Perdew, Burke, and Ernzerhof (PBE).34 To model the single layer graphene, a slab geometry is employed with a 20 Å spacing between periodic images to minimize the interaction between slabs, a 450 eV cutoﬀ for the plane-wave basis and a reciprocal space grid of size 19 × 19 × 1 for the 1 × 1 unit cell.

ASSOCIATED CONTENT S Supporting Information *

The Supporting Information is available free of charge on the ACS Publications website at DOI: 10.1021/acsnano.5b07676. 2816

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818

Article

ACS Nano

(13) Lui, C. H.; Mak, K. F.; Shan, J.; Heinz, T. F. Ultrafast Photoluminescence from Graphene. Phys. Rev. Lett. 2010, 105, 127404. (14) Reich, S.; Thomsen, C. Raman Spectroscopy of Graphite. Philos. Trans. R. Soc., A 2004, 362, 2271−2288. (15) Mostofi, A. A.; Yates, J. R.; Lee, Y.-S.; Souza, I.; Vanderbilt, D.; Marzari, N. Wannier90: a Tool for Obtaining Maximally-localised Wannier Functions. Comput. Phys. Commun. 2008, 178, 685−699. (16) Bernard, S.; Whiteway, E.; Yu, V.; Austing, D.; Hilke, M. Probing the Experimental Phonon Dispersion of Graphene Using 12C and 13C Isotopes. Phys. Rev. B: Condens. Matter Mater. Phys. 2012, 86, 085409. (17) Chen, C.-F.; Park, C.-H.; Boudouris, B. W.; Horng, J.; Geng, B.; Girit, C.; Zettl, A.; Crommie, M. F.; Segalman, R. A.; Louie, S. G.; et al. Controlling inelastic light scattering quantum pathways in graphene. Nature 2011, 471, 617−620. (18) Tan, P.; Hu, C.; Dong, J.; Shen, W.; Zhang, B. Polarization Properties, High-order Raman Spectra, and Frequency Asymmetry Between Stokes and Anti-stokes Scattering of Raman Modes in a Graphite Whisker. Phys. Rev. B: Condens. Matter Mater. Phys. 2001, 64, 214301. (19) Cançado, L.; Pimenta, M.; Saito, R.; Jorio, A.; Ladeira, L.; Grueneis, A.; Souza-Filho, A.; Dresselhaus, G.; Dresselhaus, M. Stokes and Anti-stokes Double Resonance Raman Scattering in Twodimensional Graphite. Phys. Rev. B: Condens. Matter Mater. Phys. 2002, 66, 035415. (20) Ferrari, A. C.; Basko, D. M. Raman Spectroscopy as a Versatile Tool for Studying the Properties of Graphene. Nat. Nanotechnol. 2013, 8, 235−246. (21) Berciaud, S.; Li, X.; Htoon, H.; Brus, L. E.; Doorn, S. K.; Heinz, T. F. Intrinsic Line Shape of the Raman 2d-mode in Freestanding Graphene Monolayers. Nano Lett. 2013, 13, 3517−3523. (22) Liu, H.-L.; Siregar, S.; Hasdeo, E. H.; Kumamoto, Y.; Shen, C.C.; Cheng, C.-C.; Li, L.-J.; Saito, R.; Kawata, S. Deep-ultraviolet Raman Scattering Studies of Monolayer Graphene Thin Films. Carbon 2015, 81, 807−813. (23) Schäfer-Siebert, D.; Budrowski, C.; Kuzmany, H.; Roth, S. Influence of the Conjugation Length of Polyacetylene Chains on the DC-Conductivity in Electronic Properties of Conjugated Polymers. Synth. Met. 1987, 21, 285−291. (24) Childres, I.; Jauregui, L. A.; Tian, J.; Chen, Y. P. Effect of Oxygen Plasma Etching on Graphene Studied Using Raman Spectroscopy and Electronic Transport Measurements. New J. Phys. 2011, 13, 025008. (25) Cançado, L.; Takai, K.; Enoki, T.; Endo, M.; Kim, Y.; Mizusaki, H.; Jorio, A.; Coelho, L.; Magalhaes-Paniago, R.; Pimenta, M. General Equation for the Determination of the Crystallite Size La of Nanographite by Raman Spectroscopy. Appl. Phys. Lett. 2006, 88, 163106−163106. (26) Childres, I.; Jauregui, L. A.; Park, W.; Cao, H.; Chen, Y. P. Raman Spectroscopy of Graphene and Related Materials. New J. Phys. 2013, 13, 978−981. (27) Cooper, D. R.; D’Anjou, B.; Ghattamaneni, N.; Harack, B.; Hilke, M.; Horth, A.; Majlis, N.; Massicotte, M.; Vandsburger, L.; Whiteway, E. Experimental Review of Graphene. ISRN Condens. Matter Phys. 2012, 2012, 1−56. (28) Ding, F.; Ji, H.; Chen, Y.; Herklotz, A.; Dörr, K.; Mei, Y.; Rastelli, A.; Schmidt, O. G. Stretchable Graphene: A Close Look at Fundamental Parameters Through Biaxial Straining. Nano Lett. 2010, 10, 3453−3458. (29) Rao, R.; Tishler, D.; Katoch, J.; Ishigami, M. Multiphonon Raman Scattering in Graphene. Phys. Rev. B: Condens. Matter Mater. Phys. 2011, 84, 113406. (30) May, P.; Lazzeri, M.; Venezuela, P.; Herziger, F.; Callsen, G.; Reparaz, J. S.; Hoffmann, A.; Mauri, F.; Maultzsch, J. Signature of the Two-dimensional Phonon Dispersion in Graphene Probed by Doubleresonant Raman Scattering. Phys. Rev. B: Condens. Matter Mater. Phys. 2013, 87, 075402.

(1) Time domain derivation of KHD with issues raised in the paper highlighted; (2) more discussion of oﬀresonant Raman scattering; (3) a discussion of the bandwidth outliers in Figure 8; (4) a brief review of the prior “molecular approach” to graphene (PDF)

AUTHOR INFORMATION Corresponding Author

*E-mail: [email protected]. Notes

The authors declare no competing ﬁnancial interest.

ACKNOWLEDGMENTS The authors acknowledge support from the NSF Center for Integrated Quantum Materials(CIQM) through Grant NSFDMR-1231319. We thank the Faculty of Arts and Sciences and the Department of Chemistry and Chemical Biology at Harvard University for generous partial support of this work. E.J.H. and L.K. are grateful for the hospitality and support of the Max Planck Institute for Complex Systems in Dresden in the ﬁnal stages of this work. We are indebted to Profs. Michael Hilke, Feng Wang, Yong Chen, and Philip Kim for helpful discussions and suggestions. We also thank Fikriye Idil Kaya for suggestions and a careful reading of the manuscript. We are grateful to V. Damljanovic for correcting an error concerning the multiplicity of the Γ point G mode. REFERENCES (1) Thomsen, C.; Reich, S. Double Resonant Raman Scattering in Graphite. Phys. Rev. Lett. 2000, 85, 5214. (2) Duque, J. G.; Chen, H.; Swan, A. K.; Shreve, A. P.; Kilina, S.; Tretiak, S.; Tu, X.; Zheng, M.; Doorn, S. K. Violation of the Condon Approximation in Semiconducting Carbon Nanotubes. ACS Nano 2011, 5, 5233−5241. (3) Heller, E. J.; Yang, Y.; Kocia, L. Raman Scattering in Carbon Nanosystems: Solving Polyacetylene. ACS Cent. Sci. 2015, 1, 40−49. (4) Pisana, S.; Lazzeri, M.; Casiraghi, C.; Novoselov, K. S.; Geim, A. K.; Ferrari, A. C.; Mauri, F. Breakdown of the Adiabatic BornOppenheimer Approximation in Graphene. Nat. Mater. 2007, 6, 198− 201. (5) Ferrari, A. C. Raman Spectroscopy of Graphene and Graphite: Disorder, Electron-phonon Coupling, Doping and Nonadiabatic Effects. Solid State Commun. 2007, 143, 47−57. (6) Kramers, H. A.; Heisenberg, W. Ü ber die Streuung von Strahlung durch Atome. Z. Phys. 1925, 31, 681−708. (7) Lee, S.-Y. Placzek-type Polarizability Tensors for Raman and Resonance Raman Scattering. J. Chem. Phys. 1983, 78, 723−734. (8) Dirac, P. A. M. The Quantum Theory of the Emission and Absorption of Radiation. Proc. R. Soc. London, Ser. A 1927, 114, 243− 265. (9) Beams, R.; Cançado, L. G.; Novotny, L. Low Temperature Raman Study of the Electron Coherence Length near Graphene Edges. Nano Lett. 2011, 11, 1177−1181. (10) Lucchese, M. M.; Stavale, F.; Ferreira, E. M.; Vilani, C.; Moutinho, M.; Capaz, R. B.; Achete, C.; Jorio, A. Quantifying Ioninduced Defects and Raman Relaxation Length in Graphene. Carbon 2010, 48, 1592−1597. (11) Brida, D.; Tomadin, A.; Manzoni, C.; Kim, Y. J.; Lombardo, A.; Milana, S.; Nair, R. R.; Novoselov, K.; Ferrari, A. C.; Cerullo, G.; et al. Ultrafast Collinear Scattering and Carrier Multiplication in Graphene. Nat. Commun. 2013, 4, 1−8. (12) Breusing, M.; Kuehn, S.; Winzer, T.; Malić, E.; Milde, F.; Severin, N.; Rabe, J.; Ropers, C.; Knorr, A.; Elsaesser, T. Ultrafast Nonequilibrium Carrier Dynamics in a Single Graphene Layer. Phys. Rev. B: Condens. Matter Mater. Phys. 2011, 83, 153410. 2817

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818

Article

ACS Nano (31) Lazzeri, M.; Piscanec, S.; Mauri, F.; Ferrari, A.; Robertson, J. Phonon Linewidths and Electron-phonon Coupling in Graphite and Nanotubes. Phys. Rev. B: Condens. Matter Mater. Phys. 2006, 73, 155426. (32) Kresse, G.; Furthmüller, J. Efficient Iterative Schemes for ab initio Total-energy Calculations Using a Plane-wave Basis Set. Phys. Rev. B: Condens. Matter Mater. Phys. 1996, 54, 11169. (33) Kresse, G.; Furthmüller, J. Efficiency of ab-initio Total Energy Calculations for Metals and Semiconductors Using a Plane-wave Basis Set. Comput. Mater. Sci. 1996, 6, 15−50. (34) Perdew, J. P.; Burke, K.; Ernzerhof, M. Generalized Gradient Approximation Made Simple. Phys. Rev. Lett. 1996, 77, 3865.

2818

DOI: 10.1021/acsnano.5b07676 ACS Nano 2016, 10, 2803−2818